Texture analysis of deformation induced martensite in an ... · PDF fileTheir mechanical...
Embed Size (px)
Transcript of Texture analysis of deformation induced martensite in an ... · PDF fileTheir mechanical...
Texture analysis of deformation induced martensite in an AISI 301L stainless steel: microtexture and macrotexture aspects.
Hamilton Ferreira Gomes de AbreuI, *; Marcelo Jos Gomes da SilvaI; Lus Flvio Gaspar HerculanoI; H. BhadeshiaII.
IUniversidade Federal do Cear UFC, Centro de Tecnologia, Departamento de Engenharia Metalrgica e de Materiais, Campus do Pici Bloco, 714, Pici, 60455-760 Fortaleza - CE, Brazil IIUniversity of Cambridge, Materials Science and Metallurgy, Pembroke Street, Cambridge CB2 3QZ, U.K
Abstract Experiments have been conducted to study the strain induced transformation from austenite to martensite in a metastable AISI 301LN austenitic stainless steel, deformed by uniaxial tension applied along rolling direction. Samples 10% and 20% deformed have shown the presence of ! martensite phase. Measured pole figures of martensite phase were compared to calculated ones, assuming no variant selection and selection of variants where interaction between stress and the plate of martensite adds to the driving force of transformation for favoured variants. EBSD (electron back scatter diffraction) microtexture experiments and macrotexture X-ray diffraction were performed. The orientation distribution functions (ODFs) from measured pole figure data were calculated. The measured results were compared with calculated results in both polycrystalline and single crystal samples of austenite. The results showed that the textures calculated on the basis variant selection consistent with Patel and Cohens theory, which emphasizes a mechanical component of free energy, were in good agreement with measurements. Keywords- phase transformation, texture, martensite. Introduction Metastable stainless steels are promising engineering materials due to a rewarding combination of good corrosion resistance and mechanical properties. Their mechanical properties can be affected significantly by deformation induced martensitic transformation. Furthermore, in order to use these steels to their full potential, it is important that the mechanisms acting during the martensitic phase transformation are understood from a crystallographic point of view. Deformation can induce the formation of martensite in austenitic stainless steels. The amount of martensite depends on processing parameters such as the stress state of the material, temperature and rate of deformation. The steel composition and stacking fault energy can also exert great influence (1-7). Certain stresses such as shear can induce martensitic transformation at temperatures near the martensite-start temperature (Ms). When external stresses are applied the work done contributes to the free energy change; either raising or lowering the Ms (8).
Harshad BhadeshiaMaterials Research, Vol. 12, 2009, 291-297
The interaction energy which provides the mechanical driving force for transformation is given by (8):
"GMECH = #N$ + %s (1)
where #N is the stress component normal to the habit plane, % is the shear stress resolved on the habit plane in the direction of shear and $ and s are the respective normal and shear strains associated with transformation (9). The total free energy available for transformation is the sum of chemical and mechanical components; the latter one being zero in the absence of an applied stress (10):
"G="GCHEM+ "GMECH where "GCHEM is the chemical free energy change accompanying transformation. It would be reasonable to assume that there is strong variant selection when the ratio of "GMECH/"G is large (10). The transformation sequence !"#"$, where # refers to hexagonal-close packed martensite, has been proposed for austenitic stainless steels deformed by tension and rolling by a variety of authors (11-14). On the other hand the direct transformation of austenite (!) into the body-centred cubic form $ of martensite !" $ through dislocation reactions has been found to be possible by Nolze (15). Kundu and Bhadeshia have shown that it is not necessary to consider the two-stage sequential transformation of austenite first into # and then into $ in order to calculated the transformation texture (16). In further work (17), they modelled the development of transformation texture in a deformed austenitic stainless steel using the crystallographic theory of martensite (18,19) and the interaction of austenite with applied stress following Patels and Cohens model (8). In this work, the deformation induced martensite was characterized in samples of commercial austenitic stainless steel AISI 301 LN by a combination of XRD (X-ray diffraction) and EBSD (electron backscattered diffraction) techniques. Texture evolution in austenite and martensite was studied using pole figures measured in single grains of the distinct phases, and also by representing the crystallographic texture with orientation distribution functions (ODFs) of multi-grain areas of the steel. The ODF describes the frequency of occurrence of particular orientations in an Euler space (20). The measured textures have been compared against calculations based on the crystallographic theory of martensite. Experimental In this study, a commercial AISI 301 LN stainless steel bearing 17.91Cr, 6.53Ni, 1.80 Mn, 0.79Si, 0.17Mo, 0.18Cu, 0.10N (wt%) and balance of Fe was used. Samples were solution treated for one hour at 1100oC. Specimens for tensile tests were fabricated in accordance with ASTM A370-3a standard, with 50 mm gauge length. The specimens were submitted to plastic deformations of 10%, 20% and up to rupture in a 25t-Instron machine. Figure 1 shows stress-strain curves for samples deformed 10%, 20% and deformed up to rupture. Samples for pole figure measurements by XRD and EBSD were extracted from tensile test samples from the gauge length region in accordance to figure 2.
A Philips XPert Pro X-ray diffractometer with Mo-&!% radiation tube with an attached monochromator was used for texture studies. Three incomplete pole figures for !-martensite and for austenite with maximum tilt of 75o were measured. Orientation distribution functions (ODF) were calculated in Labotex software using ADC (arbitrary defined cells) method. Three pole figures for each phase were used in the ODF calculations. Sections of '2=constant were plotted. The texture of the product resulting from ()! transformation was calculated with software crystal_habit_poly.f developed by Kundu (9) and available in the web address www.msm.cam.ac.uk/map. The EBSD studies were performed on samples from the mid plane section of the deformed region of the tensile specimens. An Oxford Crystal 300 EBSD system attached to a Philips XL-30 SEM was used and the data analysed with the aid of HKL-Channel 5 software.
Figure 1 Stress-strain curves for samples deformed 10%, 20% and ruptured.
Figure 2- Sample for tensile test with indication of areas used for X-ray pole figures and EBSD analysis.
The same crystallographic set associated with a single martensite variant for an AISI 304 stainless steel reported by Kundu (17) was used in this study. The estimated lattice parameters for austenite and martensite are 0.3589 nm and 0.2873 nm respectively. This standard set is given as follows, calculated according to reference (21): Habit plane (-0:183989 0:596344 - 0:781359)( Shape deformation matrix:
Coordinate transformation matrix :
Results Figure 3 shows an EBSD orientation map for an undeformed sample. The observed microstructure is fully austenitic and some annealing twins are vividly revealed. The fact that no colour dominates is consistent with the absence of any strong texture. Figure 4 shows orientation maps for a sample after 10% of deformation (a) austenite (b) martensite phases. After 10% of deformation, about 30% of austenite has transformed into ! martensite. White regions in Figure 4a are ! martensite. The orientation of martensite variants are in accordance with the color legend in figure 3b and can be seen in fig 4b. The stress was applied aligned with the vertical axis of the figure and martensite laths show an approximately 45o with the orientation of the applied stress. This is an indication of variant selection during martensitic transformation since the planes of maximum shear stress are located at 45o to the applied tensile stress.
(a) (b) Figure 3 (a) EBSD orientation image for undeformed sample. (b) Colour key for crystallographic orientation. HAMILTON THE MAGNIFICATION MARKERS
Figure 4 - EBSD orientation map for a sample with 10% of deformation (a) austenite (b) martensite. The orientation of the tensile stress is in the vertical direction.
Figure 5a shows the measured (100) ! pole figure for the selected grain in Figure 4b (lower right corner). Figures 5b and 5c bring the calculated pole figures applying the crystallographic theory of martensite to the parent austenite grain, assuming that 24 and or the most favoured 12 variants form, respectively. When comparing the measured pole figure to the one calculated for 12 variants, it is clear that there is a variant selection process and the Patel and Cohen model (8) seems to be a good assumption. The same procedure has been done for the 20% deformed sample (*~0.18). The selected grain is the one on the right upper corner of Figure 6a. Figure 7 shows the (100) pole figures for th